marine drugs Review
“The Good, the Bad and the Ugly” of Chitosans Barbara Bellich 1 , Ilenia D’Agostino 2 , Sabrina Semeraro 2 , Amelia Gamini 1 and Attilio Cesàro 1,3, * 1
Laboratory of Physical and Macromolecular Chemistry, Department of Chemical and Pharmaceutical Sciences, University of Trieste, Via Giorgieri 1, 34127 Trieste, Italy; [email protected]
(B.B.); [email protected]
(A.G.) Department of Life Sciences, University of Trieste, Via Giorgieri 1, 34127 Trieste, Italy; ilenia.d'[email protected]
(I.D.); [email protected]
(S.S.) Elettra-Sincrotrone Trieste, Strada Statale 14 km 163.5, Area Science Park, 34149 Trieste, Italy Correspondence: [email protected]
; Tel.: +39-040-558-3684
Academic Editors: Hitoshi Sashiwa and David Harding Received: 14 March 2016; Accepted: 9 May 2016; Published: 17 May 2016
Abstract: The objective of this paper is to emphasize the fact that while consistent interest has been paid to the industrial use of chitosan, minor attention has been devoted to spread the knowledge of a good characterization of its physico-chemical properties. Therefore, the paper attempts to critically comment on the conflicting experimental results, highlighting the facts, the myths and the controversies. The goal is to indicate how to take advantage of chitosan versatility, to learn how to manage its variability and show how to properly tackle some unexpected undesirable features. In the sections of the paper various issues that relate chitosan properties to some basic features and to advanced solutions and applications are presented. The introduction outlines some historical pioneering works, where the chemistry of chitosan was originally explored. Thereafter, particular reference is made to analytical purity, characterization and chain modifications. The macromolecular characterization is mostly related to molecular weight and to degree of acetylation, but also refers to the conformational and rheological properties and solution stability. Then, the antimicrobial activity of chitosan in relation with its solubility is reviewed. A section is dedicated to the formulation of chitosan biomaterials, from gel to nanobeads, exploring their innovative application as active carrier nanoparticles. Finally, the toxicity issue of chitosan as a polymer and as a constructed nanomaterial is briefly commented in the conclusions. Keywords: chitosan; physico-chemical properties; molecular weight; degree of acetylation; conformation; antimicrobial activity; from gel to nanobeads; drug delivery
1. Introduction Chitosan is one of the most commonly cited polymers in the scientific research dealing with a wide range of biopharmaceutical and biomedical applications including food science and technology. It has been strongly indicated as a suitable functional material in view of its excellent biocompatibility, biodegradability, non-toxicity, and adsorption properties. Originally known as a marine polysaccharide from shrimps and crabs, chitosan was primarily thought to be an easily accessible substance from the food industry waste. The original samples of chitosan were often still raw materials, with few exceptions of purification applied to chitosan in medical and cosmetic uses. The main areas in its characterization were in terms of quality (either purity or harmfulness), intrinsic macromolecular properties and physical form. Independently of the final human use, the first and most important issue was, and is still, related to the presence of impurities, metals and other inorganics, proteins, pyrogenic, endotoxic and cytotoxic agents, bioburden, all of which have received over the years erratic attention. The macromolecular characterization is mostly related to molecular weight and to degree of Mar. Drugs 2016, 14, 99; doi:10.3390/md14050099
Mar. Drugs 2016, 14, 99 Mar. Drugs 2016, 14, 99
2 of 30 2 of 31
molecular weight and to degree of acetylation, but also refers to the rheological properties and solution stability aggregation, filterability). Last, but not less important in many acetylation, but also(solubility, refers to the rheologicaland properties and solution stability (solubility, aggregation, applications, is the physical form of the powder or other morphology of the sample. Since nowadays and filterability). Last, but not less important in many applications, is the physical form of the powder orthere is a real boom of interest in chitosan, it is worth mentioning that all these characteristics have other morphology of the sample. Since nowadays there is a real boom of interest in chitosan, it is been amply and often repeatedly reported in have literature original and review articles. worth mentioning that all these characteristics beenin amply andresearch often repeatedly reported in Indeed, more than a thousand papers (1150) were published in the decade 1981–1990, increasing to literature in original research and review articles. Indeed, more than a thousand papers (1150) were more than five thousand papers (5700) in the decade 1991–2000, to about 23,100 in the first decade of published in the decade 1981–1990, increasing to more than five thousand papers (5700) in the decade this century. A current search of “Chitin and Chitosan” in research article titles gives more than 1600 1991–2000, to about 23,100 in the first decade of this century. A current search of “Chitin and Chitosan” results, almost one‐half of which were published in the last 15 years; so why write another review? in research article titles gives more than 1600 results, almost one-half of which were published in the The simple answer is that another view‐point can still be worthwhile, provided that some properties last 15 years; so why write another review? The simple answer is that another view-point can still be are cross linked and that related to properties some critical specificity chitosan novel way, specificity as reported worthwhile, provided some are cross linkedof and relatedin toa some critical of schematically in Figure 1. chitosan in a novel way, as reported schematically in Figure 1.
Figure 1. Schematic representation of relationship of chitosan properties with the pharmaceutical and Figure 1. Schematic representation of relationship of chitosan properties with the pharmaceutical and biomedical applications. biomedical applications.
Thus, having in mind to classify the “properties” of chitosan in categories as “the good, the bad Thus, having in mind to classify the “properties” of chitosan in categories as “the good, the bad and the ugly”, a scrutiny of its characteristics is here overviewed in order to introduce the theme of and the ugly”, a scrutiny of its characteristics is here overviewed in order to introduce the theme of this paper. Among all natural polysaccharides the presence of the monomer glucosamine, either fully this paper. Among all natural polysaccharides the presence of the monomer glucosamine, either fully acetylated polymers. Whether Whetherexplicitly explicitly acetylated or or partially partially deacetylated, deacetylated, isis unique unique in in the the chitin/chitosan chitin/chitosan polymers. highlighted or only mentioned as a secondary aspect, this structural characteristic is probably the basis highlighted or only mentioned as a secondary aspect, this structural characteristic is probably the ofbasis of its outstanding biophysical properties and the key for a rationale of its applications. its outstanding biophysical properties and the key for a rationale of its applications. summary, the the most most simple simple and and salient salient characteristics characteristics that InIn summary, that make make chitosan chitosan a a beneficial beneficial and and valuable polysaccharide are: valuable polysaccharide are: Chitosan isis aa linear linear natural natural polymer polymer of of glucosamine/acetylglucosamine glucosamine/acetylglucosamine that 1.1 Chitosan that behaves behaves as as a a polyelectrolyte with positive charge density at low pH. polyelectrolyte with positive charge density at low pH. Among the industrial polysaccharides, chitosan is an exception, being the only high molecular 2.2 Among the industrial polysaccharides, chitosan is an exception, being the only high molecular weight cationic polyelectrolyte, while polysaccharides are generally either neutral or anionic. weight cationic polyelectrolyte, while polysaccharides are generally either neutral or anionic. Chitosan is often claimed to be GRAS (Generally Recognized As Safe) and bioabsorbable. 3.3 Chitosan is often claimed to be GRAS (Generally Recognized As Safe) and bioabsorbable.
Mar. Drugs 2016, 14, 99
3 of 31
The same versatile “good” characteristics are indeed also the reason for several undesired effects, starting from the most obvious one when dealing with copolymers, i.e., the large variety of chemical composition in terms of comonomers. The large variety of chitosans differing in polymer size, degree of acetylation and possible chemical modifications increases exponentially. On the other hand, the simplicity of chemical modification is one of great strengths of chitosan. The “tunable” aspect of chitosan allows its optimization to give appropriate biomaterials for therapeutic applications, in principle enabling also the optimization of its biological profile. The counterpart of the structural variability is in the difficult characterization of its (statistical) distribution of comonomers (glucosamine and acetyl-glucosamine) and in the unsolved question of how the compositional variability and the molecular weight distribution add complexity to the identification of beneficial properties of the final product (the “bad”). However, the studies of chitosan uptake, distribution and toxicity are indeed quite few, since most commonly in its drug delivery formulations, chitosan is the carrier or a functional excipient. Nonetheless, it is also evident that the inspection of chitosan interactions with some co-solutes or other biostructures may reveal some subtle effects both in classical solution thermodynamics as well as in biological applications, such as the “interactions with endotoxins”. All these undesired and often hidden effects are most appropriately classified as “ugly”, because they have frustrated scientists in their research efforts. In the following sections the title issues are presented, relating and linking the chitosan properties, whenever possible, to some basic features and to advanced solutions for specific applications. Thus, after a first section in which tribute is paid to some pioneering work, the chemistry of chitosan is explored with reference, in particular, to purity, characterization issues and chain modifications. Then, the biocompatibility, antimicrobial activity and toxicity of chitosan in relation with its solution properties are reviewed. A section is dedicated to the formulation of chitosan biomaterials, from gel to nanobeads, exploring their innovative application as active carrier nanoparticles. Finally, the toxicity issue of chitosan as a polymer and as a constructed nanomaterial is briefly referred in the conclusions. Particular attention is devoted to critical comments on the various conflicting experimental results, highlighting the facts, the myths and the controversies. The goal is to make the best use of the good versatility of chitosan, to learn as much as possible how to manage its bad variability and to tackle in the proper way its ugly undesirability. 2. The Beginning A short historical annotation may usefully illustrate the continuous efforts dedicated to increasing the knowledge of chitosans in terms of structure-properties relations and therefore to improving and developing their applications. Another pertinent preliminary comment is also necessary on the link, established from the very beginning, between academic research directly or indirectly related to commercial applications and the scientists involved in the R&D of companies present on the market in the fields of either generic chemicals or, more specifically, polymers. The scrutiny of papers dealing with chitosan properties gives rise to a permanent feeling that while its “potential” is continuously stressed, for many years this seemingly remained wishful thinking. Several factors concur with the idea that using chitosan as a market product could be beneficial. Some of these will be reported in the specific application discussed in this paper. It is not strange that among the first studies on chitin and chitosan is the structural determination of the chain by diffractometry. The first X-ray diffactometric investigation of chitosan was carried out by Clark and Smith in 1936  on fibers prepared from lobster tendon chitin by a solid state N-deacetylation. A subsequent X-ray pattern was obtained and fully analyzed  with a tendon chitosan prepared from a crab tendon chitin by similar deacetylation reported by Clark and Smith. Therefore, as mentioned by Ogawa in his review  “In spite of such early finding, the pattern was analyzed in 1997 , 60 years later.” The relevance of crystallographic studies lies in the possibility that the chain conformation of chitosan can be affected by the chemical environment. Indeed, it has been shown that in the two
Mar. Drugs 2016, 14, 99
4 of 31
polymorphs, hydrated (tendon) chitosan and anhydrous (annealed) chitosan, the crystalline structures consistently present antiparallel chains in extended two-fold helix, zigzag structure, with almost constant pitches of 1.034 and 1.043 nm, for the hydrate and anhydrous forms, respectively. This chain structure is similar to those found for chitin and cellulose. However, chitosan can easily change its solid state conformation from the extended two-fold to other structures by salt formation with acids. Although not comparable with other very flexible linear polysaccharides, such as amylose and pullulan, this moderate conformational flexibility is certainly due to the presence of free amino group on the monomer residue of chitosan; thus, the advantage of chitosan for its advanced tunable applications can be envisaged. With regards to the more broad chemical and physico-chemical studies, very few papers were published on chitosan before 1970, some dealing with its characterization, a few on chemical reactions and derivative synthesis, and the largest number on its interaction with ionic species and the potential application in ion removal from waters. In this period, some research groups appear in the literature that dominated the later times. Between the 1970 and the 1980, some reactions (e.g., selective acylation) and properties of chitosan were assessed and many applicative properties of chitosan were explored. Among these works, it is particularly worth mentioning those on the hypocholesterolemic activity , the fungicidal effect , in addition to the reactions of chitosan to produce derivatives. A comprehensive review was offered by the First International Conference on Chitin/Chitosan held in 1977 in Boston , which signed the milestone for a continuous growing number of adepts in the chitin and chitosan forum. Thus, the great effort of the Muzzarelli group must be mentioned, starting with the characterization of metal chelating properties and the chromatographic uses of chitosan; as well as the contributions of the UK and Japan groups on the production and physicochemical characterization of chitosan gels. In the following decade (1981–1990), an explosion of activities all around the world in the field of carbohydrate polymers gave rise to intensive studies in this area. In parallel, there was an increase in conferences dealing with industrial application of polysaccharides, with sessions in the very large meetings (e.g., International Carbohydrate Symposium, etc.) as well as some more specific thematic meetings (e.g., Grado 1981  and Hoboken 1984 ). In the context of these meetings, several research groups emerged and the tie line for aggregation networks was marked. In these and subsequent years, while continuous efforts were made on the preparation of well-defined samples (see, for example, ), many new ideas about the use of chitosan as biomaterial became explicit and other properties of chitosan and derivatives emerged in publications. The proposed uses of chitosan included the development of artificial skin, reconstruction of periodontal tissues, hemodialysis membranes, drug targeting and many other biomedical applications. The foreseen applications were always accompanied by sentences like “this novel biomolecule, biodegradable, and biocompatible, find applications in substituting or regenerating tissues” . The similarity of chitosan structural characteristics with glycosamino-glycans, was interpreted as the reason for mimicking the functional behavior of the latter, while chitin was always structurally (or ancestrally?) associated with cellulose. In a slightly different direction, a derivative, N-carboxybutyl chitosan, was shown to display inhibitory, bactericidal, and candidacidal activities when tested against a few hundred cultures of various pathogens . It is worth remembering that the first interest in the commercial applications of chitin grew in the 1930s and early 1940s, but took a backseat for many years because of competition from synthetic polymers. Large-scale production of chitin started in the mid-1970s when regulations were introduced to limit the dumping of untreated shellfish waste in coastal waters. Chitin was easily extracted from crab, lobster and prawn shells using solvents, and the production of chitin became an economical way to comply with the regulations and dispose of thousands of tons of shellfish waste. Although chitin has applications in creams and cosmetic powders and as a material for surgical stitches, the applications of chitosan expand to a multitude of areas: antibacterial lining for bandages and wound dressings, coating for seeds to boost disease resistance, agent to prevent spoilage in winemaking, in addition to its controversial use as dietary supplement (weight-loss by avoiding fat digestion). The specific
Mar. Drugs 2016, 14, 99
5 of 31
area of food applications has been shortly reviewed in a 2016 paper , in particular for antioxidant and antimicrobial effects, which are useful in the food industry to improve food safety, quality, and shelf-life. It has been estimated that about the order of 1010 tons are produced annually by living organisms, although chitin and chitosan are recovered exclusively from marine sources. Applications of these polymers continue to grow and an estimated global market of chitin and chitosan derivative business was forecasted to exceed € 70 ˆ 109 by the year 2015 . As reported in a news agency “Not bad for bits of leftover lobster” . Before concluding this section, one point needs to be emphasized. The chain production of a ”food-waste-recycling-biopolymer” is compatible with achievement of ecological benefits and deserves further attention and effort. For chitin and chitosan, the environmentally-friendly materials produced from these renewable sources are sustainable and contribute to the creation of a circular economy, which is the current goal of an ambitious package put forward by the European Commission in December 2015 . For the more specific aspects here concerned, the waste produced each year by the shellfish processing industries represents a practical challenge, since about 75% of the total weight of crustaceans (shrimps, crabs, prawns, lobsters, and krill) ends up as by-products. The current lack of acceptable waste management options creates a potentially large environmental hazard concern. All around the world, seafood wastes are thrown away at sea, burned, landfilled, or simply left out to spoil. Therefore, the extraction of chitin from shells and its use as it is or after further processing not only is a way to minimize the waste, but also to produce compounds with valuable biological properties and specialty applications, provided that all the raw material is correctly remodeled in well characterized chemicals. As recently pointed out in literature (“don’t waste seafood waste”) , the three major components of crustacean shells are calcium carbonate (20%–50%), proteins (20%–40%) and chitin (15%–40%), which could be separated by using an integrated bio-refinery with solvent-free mechano-chemical processes. Although the main objective of this work is focused on the biopolymer chitosan, it is mandatory to mention that within this sustainability view-point, several useful chemicals and primers can be obtained from chitin [18–21], giving further value to an atom efficient economy. Once again, a parallel can also be envisaged between strategies used, or to be implemented, in cellulose and chitin exploitation. 3. A critical Examination of the Physico-Chemical Properties of Chitosan Polymers In order to emphasize, once again, the relevance of a correct understanding of the relation structure-properties in chitosan, let’s just mention in these first lines that chitosan composition has become a matter of great interest in patent claiming. Documentation for these claims lies on well-defined polymer chemical characterization and this concept will be further analyzed when discussing the difficulties encountered by regulatory agencies in approving chitosan uses. The main outcome of a critical examination of the literature results is that often (although not always!) the correlation between properties of the nanoconstructs and the structure of the macromolecular components is missed. In particular, the impression is that the advantage offered by modulating the polymer structure is turned out in the disadvantage of having final products of remarkable variability. Therefore, aiming at exploitation of chitosan and chitosan nanoparticles in modern biomedical and pharmaceutical applications, some fundamentals of physicochemical properties of this biomacromolecule cannot be overlooked. The central “dogma” is that all useful applications can in principle be traced back to three molecular determinants: the degree of acetyl substitution, the molecular weight and its distribution, the nature and the fraction of substituents as pendant groups. In the more general applications, the additional step to be examined is the interplay of these molecular characteristics with the supramolecular interactions that provide size, shape and surface properties in the nanoconstructed patterns . 3.1. Chitosan as a Copolymer: Acetylation and Substitution The first question concerns whether it is fully correct to speak about “chitosan” or better to use the term “chitosans”, making explicit the central concept that the term chitosans implies a series
Mar. Drugs 2016, 14, 99
6 of 31
of copolymers that differ not only in the fraction of comonomers but also in the distributions and clength of the comonomer sequences. This aspect is well known in polymer sciences where the terms alternate-, block- and random copolymer have been introduced. It is also the case of alginate, a close polysaccharide, where the presence along the chain of the Guluronic (G) and Mannuronic (M) monomers with varying composition and sequence type, was amply recognized since long time , allowing to conclude, from 13 CNMR studies, that the relative occurrence of G-centered triads deviated significantly from those predicted by first-order Markovian statistics . It is also known that in chitosan the two monomers, N-glucosamine and N-acetyl-glucosamine, display quite different solution properties, given the ionic character in acidic conditions of the first monomer and the slightly hydrophobic terminal in the other. This intrinsic difference, getting amplified for block-type sequences of acetyl substitution, may have dramatic consequences on chain conformation and aggregation, a fact that has encouraged the research on more hydrophobic substituents able to self-assembling and collapse in micelle-type lipospheres. Furthermore, derivatization of chitosan by grafting side chains, like is done in quaternization or glycosylation of amino groups, gives rise to a ter-polymer (namely, constituted by acetylated, de-acetylated and substituted monomers), worsening, therefore, the already complicated situation. Thus, the essential issue of chitosan composition is the proper sample characterization and, first of all, the correct determination of the degree of acetyl substituents, DA, (some authors use the term DDA, degree of de-acetylation). Over the years, several papers have referred on the determination of the degree of acetylation by physical and chemical methods, although the preferred method is often simple and easy to use, not the more accurate. The long list of methods include among all, titration [25,26], IR spectroscopy [27–31], UV spectroscopy [32,33], circular dichroism (CD) , NMR spectroscopy [35–38] and N-acetyl group hydrolysis . As a preliminary and important annotation, the comparison of data obtained with different techniques often show discrepancies in the DA values. Indeed, the difference in solubility of samples having DA from 1 (chitin) to 0 (fully deacetylated chitosan) affects sensibly the results and no single technique could be adopted to cover the full range, pointing out that solution methods can be used for soluble chitosans, whereas 13C CP/MAS NMR [36,37] and infrared spectroscopy (as recently summarized in a review ) are used for chitin and highly acetylated chitosans. Still, each method presents advantages and difficulties either in the sample preparation and/or in running the measurements. As a novel technique, the calorimetric (DSC) determination of the distinguishable decomposition of amino and acetyl groups was recently published, providing results that are independent of composition and molecular weight . Thus, DSC emerged as an accurate technique to determine the degree of N-acetylation in chitin/chitosan samples, the main advantages lying on the possibility of determining the DA in the whole 0 to 1 range, without solubilization, at lower cost in relation to NMR, and more accurately than with IR. However, all techniques, except for NMR based measurements, require an accurate weighing of chitosan. Therefore, moisture needs to be eliminated carefully and the purity of the samples must be determined separately. The degree of acetylation of chitosan determined by NMR is based on the fact that the O-Ac group is easily recognizable in the spectrum of chitosan recorded at room temperature and can be integrated and normalized by the integral either of anomeric protons or of other ring protons. More important is the possibility of generalization of the NMR method to study chitosan derivatives. An interesting application is that of glycosylated samples prepared with cellobiose, maltose and lactose residues. The glycosylation introduced a pendant made by an open sugar ring C1-linked to the amino group and C4-linked to the terminal glycosyl residue. The NMR spectra show small differences for all signals of the pendant groups except for the carbon 4 and the carbon 5, which reflect the configurational change from glucose to galactose moieties. The NMR on these samples provided a DA = 0.13 and a glycosyl substitution ratio ranging from 0.43 to 0.50 for the three derivatives . Not less important for chitosan varying in pendant group substitution is the knowledge of the substitution pattern of the groups (including the acetyl groups) along the chain, as it was referred as a relevant property in copolymers. This is illustrated in Figure 2, where it is schematically evidenced
Mar. Drugs 2016, 14, 99
7 of 31
why not only the fraction of comonomers (e.g., DA) but also their distributions and the length of the sequences of comonomers ultimately affect the polymer behavior, i.e., each copolymer species is a “specific product”. The relevance of these characteristics increases with the difference in the chemical properties of the two monomer species. Mar. Drugs 2016, 14, 99 7 of 30
Figure 2. Schematic representation of three typical patterns of monomer distribution in a copolymer, Figure 2. Schematic representation of three typical patterns of monomer distribution in a copolymer, = 0.5 should here acetylglucosamine (A) and glucosamine (B). A perfect block‐type copolymer with f here acetylglucosamine (A) and glucosamine (B). A perfect block-type copolymer Awith fA = 0.5 A value = 0 for infinite length of blocks (top). A random distribution of the monomer have a limiting p should have a limiting pA value = 0 for infinite length of blocks (top). A random distribution of that can range around 0.5. The the(middle) is characterized a limiting p monomer (middle) is characterizedA value = 0.5 for a value of f a limiting pA value = 0.5Afor a value of fA that can range alternating copolymer, by definition, should have fA = 0.5 and pA = 2 (other values evidence structural around 0.5. The alternating copolymer, by definition, should have fA = 0.5 and pA = 2 (other values irregularity). Thus, the scheme identifies limiting cases to interpret copolymer structure and evidence structural irregularity). Thus, the scheme identifies limiting cases to interpret copolymer underlines that nearest‐neighbor effects give the three copolymer structures different physico‐ structure and underlines that nearest-neighbor effects give the three copolymer structures different chemical properties. physico-chemical properties.
In general, a statistical copolymer consists of macromolecules in which the sequential In general, a statistical copolymer consists of macromolecules in which the sequential distribution distribution of the monomeric units obeys known statistical laws, such as the Markovian statistics of the monomeric units obeys known statistical laws, such as the Markovian statistics (the so-called (the so‐called random copolymer obey a zero‐order Markovian statistics, coinciding with a Bernoulli random copolymer obey a zero-order Markovian statistics, coinciding with a Bernoulli distribution of distribution of the monomers). The only very non‐random distribution of monomers is the one where themonomers monomers). very non-random distribution of be monomers is the one monomers A The and only B alternate, Poly(A‐alt‐B), which can clearly defined as where a “new” polymer, A anddifferent from Poly(A) and Poly(B) and which has rigorously fraction values f B alternate, Poly(A-alt-B), which can be clearly defined as a “new” polymer, different from Poly(A) A = fB = 0.5. Another andexample Poly(B) of and has rigorously fraction fA = fB = 0.5. Another example of a copolymer a which copolymer distribution is that values of “block copolymer” (PolyA‐block‐polyB), which is distribution is that of “block copolymer” (PolyA-block-polyB), which is characterized by sequences characterized by sequences of one monomer A interrupted by sequences of the other monomer B, the length of the sequences obeying to some n‐order Markovian statistics (with n >> 1). All these different of one monomer A interrupted by sequences of the other monomer B, the length of the sequences copolymer sequences can be initially identified the A = 1 − fB, sequences and the obeying to some n-order Markovian statistics (with by n >> 1).monomer All these fraction, different fcopolymer probability of diads, f AA , f BB , f AB . A compact mode of providing the sequence probability has been can be initially identified by the monomer fraction, fA = 1 ´ fB , and the probability of diads, fAA , fBB , fABproposed for the general case of copolymers by Bovey & Mirau  and recently used for chitosan . A compact mode of providing the sequence probability has been proposed for the general case  with the definition of the parameter p = fAB/(2fAA + fABfor ) + f AB/(2fBB + fAB). of copolymers by Bovey & Mirau  and Arecently used chitosan  with the definition of the The relevance of this quantification can be traced back to the original findings of Aiba , who parameter pA = fAB /(2fAA + fAB ) + fAB /(2fBB + fAB ). studied two samples of chitosan with similar DA but different solubility properties. This author set The relevance of this quantification can be traced back to the original findings of Aiba , up the hypothesis that the samples of chitosan with DA > 0.5 prepared from highly deacetylated who studied two samples of chitosan with similar DA but different solubility properties. This author chitin had to be considered as random‐type copolymers of N‐acetyl‐glucosamine and glucosamine set up the hypothesis that the samples of chitosan with DA > 0.5 prepared from highly deacetylated units, whereas the samples with similar DA but prepared from partial deacetylation of chitin had to chitin had to be considered as random-type copolymers of N-acetyl-glucosamine and glucosamine be considered as block‐type copolymers. units, whereas the samples with similar DA but prepared from partial deacetylation of chitin had to be In conclusion, despite some different opinions in the literature and the generally assumed considered as block-type copolymers. random statistics of residual acetyl substitution, the accurate determination of DA and of copolymer statistics is unavoidable. NMR determination of DA has been found to be precise and accurate also for the quantification of high DA, which is usually difficult to be measured with conventional techniques like IR or titration. Additionally DA can be calculated using different combinations of peaks in order to verify that the method is consistent. Some NMR techniques described in the
Mar. Drugs 2016, 14, 99
8 of 31
In conclusion, despite some different opinions in the literature and the generally assumed random statistics of residual acetyl substitution, the accurate determination of DA and of copolymer statistics is unavoidable. NMR determination of DA has been found to be precise and accurate also for the quantification of high DA, which is usually difficult to be measured with conventional techniques like IR or titration. Additionally DA can be calculated using different combinations of peaks in order to verify that the method is consistent. Some NMR techniques described in the literature are only limited by the solubility of chitosan, which depends on the DA and the molecular weight of the polymer. The relevance of DA on the solution properties of chitosan has been mentioned and, from a more general perspective, it should be stressed that all the literature results convincingly show that chain dimension and rigidity are related not only to the degree of polymerization, but also to the degree of acetylation (with a further obvious dependence upon pH and ionic strength). This point is discussed with reference to the molecular weight determination including the methods based on the knowledge of the hydrodynamic volume, having in mind the results reached on the cognate biopolymer, i.e., hyaluronan [46,47]. 3.2. Chitosan Copolymers: Molecular Weight Determination and Conformation Before reporting on molecular weight (M) determination, another subtler question arises in these data for chitosans. Not only the problem of complete solubilization (1) or even the change in the macromolecular solvation (2) affect the M measurements, but also the correct interpretation of M can be vague if the degree of substitution is not known (3). Points (1) and (2) imply solution thermodynamic issues to be reviewed, since most of the experimental methods for M determinations deal with some solution properties measurements and a dependence of the solvent goodness through the Flory interaction parameter. Point (3) is of mere analytical origin and points out on the more classical definition of macromolecular chain length in terms of degree of polymerization (DP). As an example, a monodisperse chitin sample with DP = 1000, will display a molecular weight of 203.2 ˆ 103 , while the same sample fully deacetylated, i.e., the corresponding chitosan without any degradation, has a molecular weight of 161.2 ˆ 103 , with a difference of about 20%. Therefore, even without degradation, a continuous change in the “measured” molecular weight is expected to occur upon deacetylation of chitin. This problem is much more impressive with large substituents as it occurs in the class of glycosylated chitosans [42,44]. The experimental determination of the M and M distribution of a series of samples of glycosylated chitosan with a constant DA = 0.13 and glycosyl substitution DS 0.42–0.50, is enlightening (Table 1). Table 1. Physico-chemical properties of chitosan and chitosan derivatives (reported in ). Two commercial samples of Very-Low-MW and of Low-MW and three derivatives, a trimethyl-substituted (TM-chit), a galactosyl- (Gal-chit) and a glucosyl- (Glc-chit) substituted are reported. The molecular weight of the commercial LMW sample is given to be approximately 50,000–190,000 daltons based on viscosity. TM-chit contains also substitution on O6 and O3. The sugar substituent, gal or glc, is linked to ammine via an open sugar chain, since a disaccharide is the reactant. DS (non-acetyl substitution) determined by NMR. The column “Recovery” is a parameter relevant for the data to be representative of the sample investigated. DS
VLMW-chit LMW-chit TM-chit Gal-chit Glc-chit
0.71 0.50 0.42
30 128 109 473 554
18 56 46 102 96
1.7 2.3 2.3 5.1 6.4
0.7 2.3 0.7 1.9 2.4
6.4 15.3 9.7 21.3 23.8
94 82 80 99 93
Mar. Drugs 2016, 14, 99
9 of 31
Molecular weight and conformation analysis of these derivatives were investigated at UFT—Centre for Environmental Research and Sustainable Technology, Bremen, with a “triple detectors” size exclusion chromatography Viscotek system. The array, with a differential refractometer, a right angle (90˝ ) (RALS) and a low angle (7˝ ) light scattering detector and a four capillary, differential Mar. Drugs 2016, 14, 99 9 of 30 Wheatstone bridge viscometer, provided as final data the Molecular weight (M) and Molecular Weight Distribution (MWD) of fractionated samples, including viscosity of each fraction related to a given of the viscosity, an increase (about doubling) of the molecular weight is observed in the glycosylated dilute polymer concentration . The analysis of data allow to extract the weight average Mw chitosans. This effect could be interpreted as a sign of chain dimerization, whereas simply arises from and the parameters a and k of the Mark–Houwink–Sakurada (MHS) equation (i.e., [η] = k Ma ). In particular, the most evident result is that, despite their overall similarity in the values and the trend the derivatization reaction by which a pendant with M ≈ 320 is added on the chain about every two of the viscosity, an increase (about doubling) of the molecular weight is observed in the glycosylated monomeric units, therefore doubling the original molecular weight in the absence of degradation. chitosans. This effect could be interpreted as a sign of chain dimerization, whereas simply arises from Therefore, these annotations claim for a re‐examination of many published data of chitosan samples, the derivatization reaction by which a pendant with M « 320 is added on the chain about every two in particular those with additional substitutions. monomeric units, therefore doubling the original molecular weight in the absence of degradation. As far as the conformation of chitosan with low DA is concerned, it is worth reporting that SEC Therefore, these annotations claim for a re-examination of many published data of chitosan samples, in particular those with additional substitutions. data with triple detectors provide the full plot of log [η] as a function of M with the interesting result As far as the conformation of chitosan with low DA is concerned, it is worth reporting that that the exponent coefficient a increases from 0.5 to 1 with the molecular weight decreasing from 5 × SEC data with triple detectors provide the full plot of log [η] as a function of M with the interesting 5 4 10 to 5 × 10 , in line with the independent results of Morris et al.  about the concurrent estimation result that the exponent coefficient a increases from 0.5 to 1 with the molecular weight decreasing of persistence length and mass per unit length of chitosan (Figure 3 and Table 3 of ref. ) and with from 5 ˆ 105 to 5 ˆ 104 , in line with the literature independent results (Figure 3) about the concurrent the findings for the moderately stiff hyaluronan chain. These results are collected in a sort of master estimation of persistence length and mass per unit length of chitosan (see Table 3 of ref. ) and withcontain the findings the moderately stiff hyaluronan chain. These results collected inof a sort curve and the for fundamental dependence of the exponent a as are a function the of degree of master curve and contain the fundamental dependence of the exponent a as a function of the degree of polymerization (Figure 4). polymerization (Figure 4).
Figure 3. Descriptors of the chain conformation according to the Bushin–Bohdanecky equations.
Figure 3. Descriptors of the chain conformation according to the Bushin–Bohdanecky equations. The The solutions for chitosan are described in ref . The diagram describes regions close to the target solutions for chitosan are described in ref . The diagram describes regions close to the target (dark (dark color) and regions far from the target (pale color). The white square shows the coordinates of chitosan in the persistence length Lp (nm) vs. mass-per-unit length, ML (g¨ mol´1 ¨ nm´1 ), plane color) and regions far from the target (pale color). The white square shows the coordinates of chitosan (adapted andlength redrawnLp from ref ). in the persistence (nm) vs. mass‐per‐unit length, ML (g∙mol−1∙nm−1), plane (adapted and redrawn from ref ). In conclusion, the correct polymer characterization and the robust interpretation of solution properties provide the basic knowledge for understanding the chain expansion behavior of the chitosans used for the preparation of nanoparticles, with the possibility of better tailoring the nanoparticle properties by selecting the suitable starting polymer.
Figure 3. Descriptors of the chain conformation according to the Bushin–Bohdanecky equations. The solutions for chitosan are described in ref . The diagram describes regions close to the target (dark color) and regions far from the target (pale color). The white square shows the coordinates of chitosan in the persistence length Lp (nm) vs. mass‐per‐unit length, ML (g∙mol−1∙nm−1), plane (adapted and Mar. Drugs 2016, 14, 99 10 of 31 redrawn from ref ).
Figure 4. The dependence of intrinsic viscosity of chitosan and hyaluronan as a function of degree of Figure 4. The dependence of intrinsic viscosity of chitosan and hyaluronan as a function of degree of polymerization (n) is reported as a master-plot (MHS log-log), normalized by the constant K (solvation polymerization (n) is reported as a master‐plot (MHS log‐log), normalized by the constant K constant). The emphasis is on the slope that increases with decreasing degree of polymerization n, (solvation constant). The emphasis is on the slope that increases with decreasing degree of i.e., molecular weight M. The curve is drawn with the data of Figure 6b of ref.  for hyaluronan polymerization n, i.e., molecular weight M. The curve is drawn with the data of Figure 6b of ref.  (0.5 < n < 4) and Figure 6.1 of ref  for chitosan (2 < n < 4.5). for hyaluronan (0.5